* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
198 FOOD PACKAGING TECHNOLOGY nylon 6.6 have packaging applications. It has mechanical and thermal properties similar to that of PET and therefore similar applications. PA resins can be used to make blown film, and they can be coextruded. PA can be blended with PE, PET, EVA and EVOH. It can be blow moulded to make bottles and jars which are glass clear, low in weight and have a good resistance to impact. Biaxially oriented PA film has high heat resistance and excellent resistance to stress cracking and puncture. It has good clarity and is easily thermoformed, giving a relatively deep draw. It provides a good flavour and odour barrier and is resistant to oil and fat. It has a high permeability to moisture vapour and is difficult to heat seal. These features can be overcome by PVdC coating. They can also be overcome by lamination or coextrusion with polyethylene, and this structure is used as the bottom thermoformable web, i.e. deep drawn, for packing bacon and cheese in vacuum packs or in gas-flushed packs (MAP or modified atmosphere packaging). The film can be metallised. PA film is used in retortable packaging in structures such as PA/aluminium foil/PP. The film is non-whitening in retort processing. PA is relatively expensive compared with, for example, PE, but as it has superior properties, it is effective in low thicknesses. 7.3.9 Polyvinyl chloride (PVC) If one of the hydrogen atoms in ethylene is replaced with a chlorine atom, the resultant molecule is called vinyl chloride monomer (VCM). Addition polymerisation of vinyl chloride produces PVC. Unplasticised PVC (UPVC) has useful properties but is a hard, brittle material, and modification is necessary for it to be used successfully. Flexibility can be achieved by the inclusion of plasticisers, reduced surface friction with slip agents, various colours by the addition of pigments and improved thermal processing by the addition of stabilising agents. Care must be exercised in the choice of additives used in film which will be in direct contact with food, particularly with respect to the migration of packaging components into foodstuffs. Rigid UPVC is used for transparent or coloured compartmented trays for chocolate assortments and biscuits. It is used with MAP for thermoformed trays to pack salads, sandwiches and cooked meats. Most PVC films are produced by extrusion, using the bubble process. It can be oriented to produce film with a high degree of shrinkability. Up to 50% shrinkage is possible at quite low temperatures. The film releases the lowest energy of the commonly used plastic films when it is heat shrunk around products. It is plasticised, and the high stretch and cling make it suitable for overwrapping fresh produce, e.g. apples and meat in rigid trays using semi-automatic and manual methods.